**HAL Id: hal-00879265**

**https://hal-mines-paristech.archives-ouvertes.fr/hal-00879265**

Submitted on 2 Nov 2013

**HAL is a multi-disciplinary open access**
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Estimation of Acoustic Properties, of the Representative**

**Volume Element of Random Fibrous Media**

### Charles Peyrega, Dominique Jeulin

**To cite this version:**

Charles Peyrega, Dominique Jeulin. Estimation of Acoustic Properties, of the Representative Volume Element of Random Fibrous Media. Journal of Applied Physics, American Institute of Physics, 2013, 113 (10), pp.104901-104901-13. �hal-00879265�

### Estimation of acoustic properties and of the representative volume element

### of random fibrous media

Charles Peyrega and Dominique Jeulin

Citation: J. Appl. Phys. 113, 104901 (2013); doi: 10.1063/1.4794501 View online: http://dx.doi.org/10.1063/1.4794501

View Table of Contents: http://jap.aip.org/resource/1/JAPIAU/v113/i10

Published by the American Institute of Physics.

### Related Articles

Influence of working liquid on the onset characteristics of a thermoacoustic engine with gas and liquid

J. Appl. Phys. 112, 094909 (2012)

Comprehensive characterization of thermophysical properties in solids using thermal impedance

J. Appl. Phys. 112, 094901 (2012)

Variable-thickness multilayered polyvinylidene fluoride transducer with improved sensitivity and bandwidth for photoacoustic imaging

Appl. Phys. Lett. 101, 173702 (2012)

Nonlinear acoustic impedance of thermoacoustic stack

J. Appl. Phys. 112, 063518 (2012)

Spectroscopic thermoacoustic imaging of water and fat composition

Appl. Phys. Lett. 101, 033705 (2012)

### Additional information on J. Appl. Phys.

Journal Homepage: http://jap.aip.org/Journal Information: http://jap.aip.org/about/about_the_journal

Top downloads: http://jap.aip.org/features/most_downloaded

### Estimation of acoustic properties and of the representative volume element

### of random fibrous media

Charles Peyregaa)and Dominique Jeulina)

Centre de Morphologie Mathematique, Mathematiques et Syste`mes, Mines ParisTech, 35 rue Saint Honore, 77300 Fontainebleau, France

(Received 10 July 2012; accepted 21 February 2013; published online 11 March 2013)

This work focuses on the estimation of acoustic properties from numerical simulations, and on the determination of the representative volume element of random fibrous media. At the microscopic scale, both viscous and thermal dissipations of energy occur in the air saturating the pores of a porous medium. Thus, the thermoacoustic formalism was used to model the physical behavior of several periodic unit cells of random fibrous media. Their properties such as both harmonic acoustic velocity and temperature were homogenized at different scales, in order to estimate representative volume elements for different properties. VC 2013 American Institute of Physics.

[http://dx.doi.org/10.1063/1.4794501]

I. INTRODUCTION

For engineering purpose, predicting acoustic properties of random media from their microstructure is a first step to design new materials with improved properties, like a better sound attenuation. One of the challenging problems to solve concerns the fluctuations of the microstructure and of the local physical fields involved in the homogenization of the acoustic behaviour.

This work was inspired by previous studies made in the framework of the Silent Wall project, with a main objective, which consisted in designing an insulating system using fi-brous media with optimized acoustic absorption properties. Several results are available in previous publications (Refs.

32–34) and will not be detailed in this paper. The main method, we used to estimate the acoustic behaviour of fi-brous media was based on finite element simulations over periodic unit cells of regularly distributed parallel fibres. This paper focuses on the acoustic absorption properties of fibrous media composed of randomly distributed fibres, in order to estimate the characteristic sizes of the simulated acoustic fields. Finally, the main objective of this work con-sists in defining the representative volume element of such random cells to estimate the coefficient of acoustic absorp-tion with a controlled statistical precision.

II. MODELLING THERMOACOUSTICS A. The thermoacoustic equations

Our work highlights the macroscopic properties of fi-brous media from their behaviour at the microscopic scale, by simulating their thermo-acoustic properties, in order to correctly handle the viscous and thermal dissipation of the acoustic energy.14,21,28,32,41 Starting from three harmonic variables: the flow velocity ~U (Eq. (1)), the pressure P (Eq.

(2)), and the temperature of the fluidT (Eq.(3)), we consider

their variations, respectively, defined as acoustic velocity~u, pressurep, and temperature s.

~

U¼ ~U0þ ~u ei x t; (1)

P¼ P0þ p ei x t; (2)

T ¼ T0þ s ei x t: (3)

Four fully coupled equations are solved: the equation of Navier Stokes (Eq.(4)), the equation of continuity (Eq.(5)), the heat equation (Eq. (6)), and finally the equation of the perfect gases (Eq. (7)) inside the pores saturated by air. The air is considered as a visco-thermal fluid and as a perfect gas at the microscopic scale. The ambient pressure and tempera-ture are, respectively, defined asP0andT0.

i x q0~u ¼ ~rp þ
g
3þ f
~
rð ~r:~u_{Þ þ g D~}u; (4)
i x q
q0
þ ~r:~u ¼ 0; (5)
i x q0Cp s¼ j Ds þ i x p; (6)
qðp; sÞjP0;T0 ¼ q0
p
P0
s
T0
: (7)

Moreover, our study is made in the framework of the formalism proposed by Refs.1,3, and18, which considers a porous medium as an equivalent fluid with a rigid skeleton (here the fibrous network). Thus, the interface C between fibres and pores is considered as an adiabatic rigid boundary, which implies both acoustic velocity~u (Eq.(8)) and temper-ature s (Eq.(9)) equal to zero onC.

~u_{C}¼ ~0; (8)

s_{C}¼ 0: (9)

a)_{Electronic} _{mail} _{addresses:} _{Charles.Peyrega@mines-paristech.fr} _{and}

Dominique.Jeulin@mines-paristech.fr. URL:http://cmm.ensmp.fr/.

0021-8979/2013/113(10)/104901/13/$30.00 _{113, 104901-1} VC_{2013 American Institute of Physics}

B. Homogenization of periodic structures in acoustics

In order to estimate, the macroscopic acoustic proper-ties of a porous medium from its physical behaviour at the microscopic scale, we use the theory of the homogenization of periodic structures.5–7,39,40 This method was handled in our previous work concerning the thermoacoustic modelling of fibrous media (Refs. 32–34), and was inspired from different studies concerning different porous materials (Refs.15,21,22,28,30,37, and41).

The three complex acoustic variables ~u; p; and s are X periodic on the boundaries C of the cells defined into the domainX. According to this method these three var-iables can be expressed from a multi-scale point of view.15,21,22,28–34,41,42 Considering a periodic microscopic unit cellX, it is possible to estimate the acoustic absorption of the corresponding fibre board from the effective tensor of dynamic viscous permeability K and from the effective sca-lar thermal permeability K0 of this cell, assuming that viscous and thermal phenomena can be handled separately.1,3,8–10,12,18,20,25–27,38,44 The local values of K andK0 in the microscopic cell are, respectively, estimated from the Eq.(10)(the Darcy’s law) and the Eq.(11).

uð0Þ
!
ð~x;~yÞ ¼ Kð~y; xÞ
g :!prx
ð0Þ_{ð~}_{xÞ;}
(10)
sð0Þð~x;~yÞ ¼K
0_{ð~}_{y; xÞ}
j i x p
ð0Þ_{ð~}_{xÞ:} _{(11)}

As explained in Refs. 18,20–22, and38, the multiscale approach links the macroscopic and the microscopic acoustic properties of our fibrous medium, respectively, characterized by two spatial variables notedx and y. Thus, from a separa-tion of scales, we note !pðxÞ the gradient of the macro-rx

scopic pressure in the material which is assumed to be constant at the microscopic scale.21,22Therefore, the acoustic pressure is assumed to be a macroscopic variable only depending on the macroscopic spatial variable x. We can notice that both K andK0 are locally defined at the micro-scopic scaley and depend on the frequency X of the acoustic propagating wave. Let for instancepðxÞ ¼ 1 Pa be the con-stant amplitude of the macroscopic acoustic pressure applied to the fibrous material.

C. Macroscopic acoustic properties of homogenized porous media

As an illustration for this method, we first consider in Fig.1an infinite layer in 3D having a thickness equal tod. This layer is composed of a periodic pattern of parallel regu-larly distributed fibres (called PACC: periodic array of circu-lar cylinders, according to Ref.41), and is stimulated by an incoming propagating acoustic wave, which splits into a reflected wave and an absorbed wave. In our work our objec-tive consists in optimizing the acoustic properties of such a medium by increasing the fraction of the incoming wave absorbed by the material.

Let K andK0, respectively, be the effective viscous per-meability and the effective thermal perper-meability of the full

X unit periodic cell Fig.2(i.e., over both porous and fibrous phases).

In order to estimate, the acoustic properties of such a fi-brous medium, we solved the thermoacoustic equations pre-sented in Sec. II A with the finite element software Comsol MultiphysicsTM,11 for different frequencies between 0 Hz and 4032 Hz. Only the pores around the rigid fibre are meshed into Fig. 2, but we consider both Eqs.(8)and(9)in the fibrous phase (central white disc). Moreover, the mesh at the interface C was refined in order to properly solve the equations in the boundary layer (more details are given in Sec.II D)). We note qeffthe effective tensor of density of the

macroscopic equivalent medium, which is estimated by below equation

q_{eff} ¼g /
i xK

1_{:}

(12) Then, we estimate the effective scalar compressibility modulus veff (Eq. (13)), with Pr the Prandtl number of the

air, and c¼ 1:4, the perfect gas constant.

FIG. 1. 3D equivalent infinite layer (along Oy and Oz) of homogenized material composed of elementary periodic unit cells PACC (fibres with circular cross section) having a thickness equal tod along Ox. Stimulation alongOx. Red square: 2D unit cell (Fig.2).

FIG. 2. 2D PACC 64 meshed periodic unit cell representing a cross section of the geometry in Fig.1. Only the pores are meshed with a porosityU ¼ 0:64.

v_{eff}ðxÞ ¼ 1
cP0
c ðc 1Þq0Pr
g
i x K0
/
: (13)

Considering ~Q¼ Q~n the wave vector defined from the
unit vector ~n and parameters q_{eff} and veff, we can estimate

the effective characteristic velocity ceff (Eq. (14)) and the

effective characteristic acoustic impedanceZceff(Eq.(15)) of the homogenized porous medium.

ceff ¼
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
nT
!
qeff1~n
v_{eff} ¼
x
Q;
v
u
u
t _{(14)}
Zceff ¼
1
/
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ
nT
!
qeff~n
v_{eff} :
v
u
u
t _{(15)}

Finally, parameters q_{eff} and v_{eff} can be used to calculate
the acoustic impedanceZd(Eq. (16)) of a macroscopic
me-dium having a thickness equal tod (Fig.1).

Zd ¼ Zceff

1þ eð2 i x dceff Þ

1 eð2 i x dceff Þ

" #

: (16)

The coefficient of reflection RðxÞ (Eq. (17)) is a com-plex number estimated fromZdand fromZ0 ¼ q0c0, the

im-pedance of the air saturating the pores, and leads to the coefficient of absorptionAðxÞ (Eq.(18)) of the correspond-ing d-thick macroscopic material.

RðxÞ ¼Zd Z0 Zdþ Z0

; (17)

aðxÞ ¼ 1 jRðxÞj2: (18)

D. Macroscopic acoustic properties of deterministic fibrous media

In previous works, using image processing methods like mathematical morphology (Refs. 32, 35, and 36), we have highlighted some morphological properties of the ThermisorelTMat the microscopic scale, such as its external porosityU ¼ 0:64 and its volume weighted average radius RF¼ 42 lm. The 3D microstructure of this fibrous material

is illustrated in Fig.3with a 3D tomographic X-Ray image. In the further experimental results concerning the ThermisorelTM, the acoustic stimulation is made along the Oz axis, perpendicularly to the fibres which are isotropi-cally oriented in thexOy planes.

For instance, Fig.4shows that a 4 cm thick fibre board like the ThermisorelTM(black and green plots) has a similar acoustic absorption coefficient as the simulated determinis-tic medium composed of 2D PACC 64 periodic unit cells (Fig.2) with a radius equal toRF¼ 42 lm (orange plot), in

the frequency range between 53 Hz and 4032 Hz. Note that the homogenized acoustic absorption coefficient is obtained without any experimental fitting from measurements. The experimental acoustic absorption of the ThermisorelTMwas

measured by the LAUM (Laboratoire d’Acoustique de l’Universite du Maine, Le Mans, France) with a Kundt’s tube.

Note that the two peaks of absorption around 2500 Hz in Fig. 4 are measurement artefacts due to the vibration resonances of the Kundt’s tube used to measure aðxÞ, and therefore are not significant. In Fig. 4, we can observe to what extent the size of the fibre radii influences the absorp-tion coefficient of a fibre board with a given porosity (here U ¼ 0:64) and thickness (here d ¼ 4 cm).

These results are more detailed in our previous publica-tions on this topic (Refs.32–34), where it was shown to what extent a compromise should be found between small and large fibres. Decreasing the radius of the fibres for a given porosityU implies an increase of the specific surface area Sv of the fibres-pores interface, expressed inm1. According to

FIG. 3. 3D X-Ray CT image of ThermisorelTM. Resolution: 15lm=voxel.

FIG. 4. Acoustic absorption coefficients of single layered materials com-posed of 2D PACC cells with a porosityU ¼ 0:64, for different fibre radii, and having a thicknessd equal to 4 cm, for f between 53 Hz and 4032 Hz. Comparison to the experimental properties of ThermisorelTM (Source: LAUM).

the Eq.(19), the specific surface area is the ratio between the surface of the fibres-pores interfaceS and the total volume of the sample.

Sv¼

S VTotal

: (19)

In acoustics, the dissipation of energy occurs at this interface, in the so-called boundary layer, whose thickness dBL is directly linked to the frequency of the propagating

sound wave, according to the Eq.(20).1,2Thus, the lower the
frequency the thicker the boundary layer. That is, why the
fi-nite element mesh of the microstructures has to be refined at
the interface of the fibres (Fig. 2), in order to properly
resolve the thermoacoustic equations in the boundary layer,
and then to correctly estimate the acoustic properties of the
cell.
dBL¼
ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ_{g}
f p q0
r
: (20)

Knowing the relationship between the thickness dBL and

the frequency f, we observed that reducing the radius RF implies an increasing surface areaSvfor a given pore volume fraction, and then a global increasing acoustic absorption in the frequency range (cf. plots forRF¼ 200 lm (blue plot)

andRF¼ 100 lm (pink plot) in Fig.4). However, reducing

the size of the fibres too much, with a constant pore volume fraction U, will cause an observable drop of the acoustic absorption coefficient (cf. plots for RF¼ 80 lm (black

dashed plot) toRF¼ 20 lm (gray dashed plot) in Fig.4).

III. RANDOM FIBROUS MEDIA

A. Acoustic fields simulated on random unit cells

In the Sec.II Cwas introduced a computational method to simulate the thermoacoustic behaviour of a deterministic fibrous medium. In this section, we will focus on the acoustic properties of random fibrous media, since the microstructure of the ThermisorelTMis heterogeneous. In previous publica-tions, a morphological model was proposed to represent 3D virtual fibrous materials with morphological properties simi-lar to the ThermisorelTM. Based on the theory of random sets (Refs.16and23), our method makes use of a Boolean model of random cylinders with random radii, lengths and orienta-tions in 3D.32,35Since the theoretical morphological proper-ties of the random Boolean model are known, it is possible to make an identification of the model from image analysis measurements.

In this study, we have chosen to model random fibrous media by infinite parallel fibres, like 2D PACC cells in Fig.1, but randomly distributed in 3D, with cross sections represent-ing a Boolean model of discs. We will call these geometries 2D PACC RANDOM. The Fig.5 shows the static fields of acoustic velocity in two unit cells (1 and 2) amongn¼ 20 in-dependent realizations, composed of overlapping fibres in ac-cordance with the Boolean model, as the result of the location of the centres of discs, according to a random Poisson point process.16,23These unit cellsX are X periodic, which

means that the three acoustic fields~u; p; s, and even the geo-metries of their microstructures, are periodic in both Ox and Oy directions. Moreover, all the fibres have the same radius (hereRF¼ 42 lm).

Their pore volume fractions are respectively equal to UA ¼ 0:65 and UB ¼ 0:66. This fluctuation is a result of the

Poisson point process driving the Boolean model (Refs. 23,

32, and 35) which implies random pore volume fractions around the average valueUAVG¼ 0:64. This study is different

from our previous work concerning the acoustic properties of random fibrous media (Refs.32and 34) because the consid-ered microstructures were especially chosen for having a con-stant pore volume fraction (0.64). Thus, only the effects of the geometrical fluctuations at constant porosity were studied.

The absolute value of the complex harmonic acoustic fieldsjsj of the simulation 1 are represented in Fig.6for fre-quencies in the range 53 Hz–1126 Hz, at two different scales:

FIG. 5. Static fields of acoustic velocity~u (m/s) (f¼ 0 Hz) for two periodic el-ementary unit cells (among 20 independent realizations). Acoustic stimulation in the verticalOy direction, sources at the top of the geometries. RF¼ 42 lm.

RF¼ 42 lm and 100 lm. Note that the square geometries at

these two different scales are obtained with homothetic trans-formations, which are quantitatively described in the TableI, where the side lengths lC and surface areas AC of the 2D PACC RANDOM cells are listed for each scale of radiusRF.

Like in our previous work (Refs. 32–34), we can observe that the boundary layer (blue areas with jsj 0 at theC air-fibre interface) gets thinner at high frequency, and that an overlap of neighboring boundary layers is seen at low frequencies for small fibres.

Generally speaking, both acoustic fields~u and s, respec-tively, represented in Figs. 5 and 6, are not homogeneous and local fluctuations appear. This directly influences the variations of the acoustic properties between realizations.

B. Macroscopic acoustic properties of random fibrous media

After having simulated the thermoacoustic behaviour of n¼ 20 independent microstructures of periodic random fi-brous media at three different scales RF¼ 42 lm; 100 lm;

and 300 lm (which implies a total of 3 20 ¼ 60
computa-tional simulations), the next step consisted in estimating the
average absorption coefficientEfaðxÞg obtained from n ¼ 20
independent realizations for each scale and for a given
thick-ness (here d¼ 2 cm; 4 cm, and 10 cm). For each radius RF,
the average absorption coefficient in Fig. 7 was estimated
from both permeabilitiesEfKg and EfK0_{g averaged over the}

n¼ 20 independent periodic microstructures and injected in the equations in Sec.II C.

In Fig.7, the acoustic absorption of fibre boards com-posed of deterministic 2D PACC unit cells (in orange) are compared to the average absorption coefficient EfaðxÞg (in green) obtained from then¼ 20 2D PACC RANDOM peri-odic microstructures for the cased¼ 4 cm, the conclusions derived from other thicknesses being similar. At first sight, we can observe that deterministic and random cells do not give exactly the same absorption coefficients, but they are close. For example, deterministic and random geometries with radii equal to RF ¼ 42 lm have very similar acoustic

absorption coefficients in the full frequency range. For larger fibres (RF¼ 100 lm and 300 lm) the frequency evolutions

are globally similar with almost identical amplitudes, but a so-called “frequency shift” is observed between regular and random microstructures.

The blue dots in Fig.7represent the absorption coeffi-cient of each experimental simulation (amongn¼ 20). Thus, we can observe that for large fibres (RF¼ 300 lm), the

fluc-tuations of the absorption coefficient are high.

FIG. 6. Harmonic fields of acoustic temperature s (K) for three frequenciesf between 53 Hz and 1126 Hz for the periodic elementary unit cell 1 at different scales (RF¼ 42 lm and 100 lm). Acoustic stimulation in the vertical Oy direction, sources at the top of the geometries. In this illustration, the configuration of fibres is kept constant, while changing their diameter.

TABLE I. LengthslC(in mm) and surface areasAC (in mm2) of the 2D

PACC RANDOM unit cells for the different fibre radiiRF(in lm).

RF 42 lm 100 lm 300 lm

lCðmmÞ 2.52 6 18

ACðmm2Þ 6.35 36 324

IV. ESTIMATION OF THE REPRESENTATIVE VOLUME ELEMENT

A. General method

The fluctuations of aðxÞ observed throughout the n ¼ 20 realizations in Fig.7can be quantified in order to define the relative precision to estimate the average absorption coeffi-cientEfaðxÞg over the n ¼ 20 independent realizations, hav-ing a surface areaAC(TableI).

In this section, we will present a method to estimate the representative volume element of such a material for differ-ent physical properties. The main objective consists in defin-ing the minimum volume for which the properties remain stable, whatever the random sample considered. For this pur-pose the fluctuations of different acoustic fields (velocity, temperature, and absorption) are studied fromn independent unit cells composed of randomly distributed fibres.

In order to determine the relative precision of the
esti-mation of an effective physical propertyhZi, obtained from
n independent random microstructures, each one having a
surface area equal toAC, it is necessary to estimate the
var-ianceVARðhZiÞ of the random variable hZi over the n
inde-pendent unit cells. The relative precision is defined from
the 95% estimation error95%(Eqs.(21)and(22)), deduced
from the 95% confidence intervalhZi695%inside which the
exact average valueEfhZig is contained with a probability
0:95; EfhZig being the average of hZi over the n realizations
of the cell.
2
95%¼
4 VARðhZi_{A}_{C}Þ
n ; (21)
2 _{¼}
2
95%
EfhZig2: (22)

It is known (Refs.4,13,17,19,24, and43), that the var-ianceVARðhZiÞ can be expressed by Eq.(23), as a function of the point varianceVARðZÞ and of the integral range A2, namely the integral of the correlation function, as defined by Eq.(27)below, measuring the scale of the fluctuations of the average physical propertyhZi. Noting A the surface area of the individual cells, we asymptotically obtain the Eq.(23)

forA A2.

VARðhZi_{A}Þ
VARðZÞ ¼ A2

1

A: (23)

Thus, the relative precision of the estimation of hZi, obtained from n independent unit cells with a surface area equal to A¼ AC (Eq. (24)), can be deduced from Eqs.

(21)–(23)if the conditionA A2is satisfied.

2_{¼} 4 VARðZÞ A2

n AC EfhZig

2: (24)

In order to estimate the integral rangeA2, the method we used consists in calculating the varianceVARðhZiÞ of the av-erage property hZi over all the disjointed subareas A of the domain A0 ¼ n AC. Moreover, we noteVARðZÞ the point

variance of the random propertyZ over the total surface area A0of the n microstructures. The use of Eq. (23)was vali-dated in many previous studies (see Refs.4,13,19, and43, among others). A further validation is made here on the fluc-tuations of the area fraction, as explained at the end of Sec.

IV B 1 and by comparison between theoretical and experi-mental results (TableII).

To illustrate this method, the Fig.8represents the effec-tive acoustic velocity averaged over subareas of the micro-structure 1 for different ratios (1;1

4; and 1 9Þ.

Finally, the representative volume elementARVE, into

which the average value hZi of the random variable Z is estimated with a relative precision , is defined in Eq.

(25).4,13,17,19,43 The Eq. (25) is defined from the Eq.(24), withn¼ 1 and A2estimated from Eq.(23).

ARVE ¼

4 VARðZÞ A2

2_{ EfhZig}2 : (25)

B. Representative volume element of the microstructure

1. Integral range of the microstructure

Using the method presented in the Sec.IV A, we consider now as a random functionZ(x), the indicator function of the pores (ZðxÞ ¼ 1 when x is located inside the pores, and ZðxÞ ¼ 0 in the fibres). In that case, the value VARðZÞ in the

FIG. 7. Comparison of the absorption coefficient of regular 2D PACC 64 homogenized microstructures to the average absorption coefficient (ingreen) of the 20 independent homogenized random fibrous media (individual absorption inblue) having a thickness d equal to 4 cm, for f between 53 Hz and 4032 Hz. RF¼ 42 lm; 100 lm, and 300 lm.

Eq. (23) is given by the equation: VARðZÞ ¼ U ð1 UÞ, withU the area fraction of the pores.

Let CðhÞ be the centered covariance of a stationary random variable Z with mathematical expectation EfZg (Eq.(26)).24We have

CðhÞ ¼ EfðZðxÞ EfZgÞ ðZðx þ hÞ EfZgÞg: (26)
For the indicator function, we can write the following
equation: C_{ðhÞ ¼ QðhÞ U}2 _{¼ CðhÞ ð1 UÞ}2, withCðhÞ
and QðhÞ the covariances, respectively, of the fibres and of
the pores. By definition, we have CðhÞ ¼ Pfx 2 fibres;
xþ h 2 fibresg, while QðhÞ ¼ Pfx 2 pores; x þ h 2 pores g.
Then, the integral range A2can be obtained as a function of

CðhÞ into the below equation A2 ¼ 1 U ð1 UÞ ð <2 CðhÞdh: (27)

The random microstructures used for the simulations are Boolean models of random discs, which represent random fi-brous media. They are obtained by implantation of discs with a random radiusR (here, we have R¼ RF) on random

points xk of a Poisson point process. Realizations of the model are shown on Figs. 5,6, and8, where it is clear that overlaps between discs are allowed, as a result of the Poisson point process, where points are located at random, without any interaction. Thus, CðhÞ can be analytically defined by the theoretical expression QBDðhÞ of the covariance QðhÞ of

the pores of a Boolean model of discs (noted BD) defined below.16,23,32,35

QBDðhÞ ¼ Uð2rDðhÞÞ: (28)

We noterDðhÞ, the normalized geometrical covariogram

of a disc. The geometrical covariogram of any random pri-mary grainX0and its normalized geometric covariogram are respectively defined by the Eqs.(29)and(30), ln being the

average volume in 3D or the average area in 2D of the ran-dom grainsX0, over then realizations.

KðhÞ ¼ lnðX0\ XhÞ; (29)

rðhÞ ¼KðhÞ Kð0Þ¼

KðhÞ

l_{n}ðX0_{Þ}: (30)

Considering discs as primary grains having a constant radius r, we can note their geometrical covariogram as KDðh; rÞ ¼ 0 if h > 2r. It is obtained as the area of the

inter-section of two discs with the same radiusr when their centres are separated by distanceh. The Eq.(31)gives by geometri-cal geometri-calculation the values ofKDðh; rÞ when 0 h 2r.

KDðh; rÞ ¼ 2r2 arccos h 2r h 2r ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 h 2r 2 s 0 @ 1 A: (31)

Then, from Eqs.(28),(30), and(31)into the Eq.(27), it is possible to compute the theoretical integral rangeA2BDof a

Boolean model of random discs (Eq.(32)).

FIG. 8. Average acoustic velocity over subareas of the microstructure 1 for different surface ratios (1;1

4; and 1

9Þ. Acoustic stimulation in the vertical Oy direction, source at the top of the geometry.

A2BD ¼
4p
VARðZÞ
ð2RF
h¼0
h CBDðhÞ dh
A2BD ¼
4p
VARðZÞ
ð2RF
h¼0
hQBDðhÞ U2
dh
A2BD ¼
4p
VARðZÞ
ð2RF
h¼0
hU
2rDðhÞ
U2_{dh:}
8
>
>
>
>
>
>
>
>
>
<
>
>
>
>
>
>
>
>
>
:
(32)

Using the Eq. (23), the integral rangeA2of the
micro-structure (i.e., of the porosity) was estimated from a linear
regression of the functionVAR_{ðhUi}_{A}_{Þ=VARðUÞ with respect}
toð1=AÞ. The function VARðhUiAÞ was calculated by

split-ting the 20 realizations of 2D PACC RANDOM unit cells into equal disjointed subareas with differentA surface areas (Fig. 8). The Fig. 9 shows this linear regression over the scales 1 to 8 (i.e., over the surface ratios 1 to 1/64) in loga-rithmic scales for both axis for the caseRF¼ 42 lm.

The resulting integral rangeA2is compared to the theo-retical one (Eq.(24)) in the TableII. The theoretical values and the estimated values differ with a relative error close to 20% of the theoretical ones.

2. RVE of the porosity

After having estimated the integral range A2 of the average porosity from n¼ 20 realizations in Sec. IV B 1

(TableII), we can estimate from the Eq.(25)the representa-tive volume element ARVE for which the average porosity

hUi is known with the relative precision . On the Fig.10, is given the evolution of the relative precision of estimation of

hUi as a function of the surface area A of one random realiza-tion (n¼ 1) at different scales (RF ¼ 42 lm; 100 lm, and

300 lm). It enables us to estimate the representative element ARVE for a specific precision. The minimum surface area A

on theOx axis is equal to ACin TableI, which shows that a single realization like those simulated in our work provides an estimatehUi with a relative precision hUi¼ 3:7%.

According to the Eq.(24), the relative precision of the estimation ofhUi for the 20 images is equal to hUi¼ 0:83%,

which shows that both number (n¼ 20) and size (AC) of images (Table I) are representative enough to estimate the average porosityhUi with a very good precision. This con-clusion is validated by the fact that the linear range for which

FIG. 9. Estimation of the integral rangeA2ðPorosityÞ of n ¼ 20 independ-ent microstructures (Boolean model of random discs) for RF¼ 42 lm. Logarithmic scales.

FIG. 10. Evolution of the relative precision of estimation ofhUi over the surface area A of one random realization (n¼ 1) at different scales (RF¼ 42 lm; 100 lm; and 300 lm). The minimum surface area A on the Ox axis is equal toACin TableI. Blue dashed vertical line:¼ 1 %. Logarithmic

scales.

TABLE II. Comparison betweenA2Simu estimated over 20 microstructures,

and the theoretical integral rangeA2BDof an infinite Boolean model of

ran-dom discs with a radiusRF.

RFðlmÞ A2Simuðmm
2_{Þ} _{A}
2BDðmm
2_{Þ}
42 0.0039 0.0049
100 0.0222 0.0277
300 0.1995 0.2495

A A2 is relatively large in Fig. 9, since the linear

regres-sion ofVARðhUiAÞ=VARðUÞ, according to ð1=AÞ was

calcu-lated over the 8 first area ratios (from 1 to 1/64).

C. Representative volume element of complex acoustic fields

1. Integral range of complex acoustic fields

Since both variables~u and s are complex, our study sepa-rately focuses on the respective real and imaginary parts of these two variables. Thus, the estimation of the RVE handles the following four fields: Re½~u; Im½~u; Re½s, and Im½s. Moreover, we consider the random scalar fields Re½uy;

Im½uy; Re½s; and Im½s as random functions. We note uythe scalar complex component of~u along Oy, because the acoustic stimulation is only oriented along this direction (Figs.5and6). Using the method presented in Sec. IV B 1, we estimate A2for each of these four random fieldsZ(x), as shown in Fig.

11forRF¼ 42 lm. We can observe that the linear regressions

of both componentsRe½uy and Im½uy of the acoustic velocity,

were made on the first 5 surface ratios (1;1 4; 1 9; 1 16, and 1 25) for

which the linear approximation expressed in Eq.(23)can be made according to the conditionA A2. However, the

inte-gral ranges of the two components of the acoustic temperature s were estimated from linear regressions on the first 3 surface ratios (1;1

4; and 1

9), which shows that the linear range, for

whichA A2is satisfied, is barely reached for our 20 images

with surface area equal toAC(TableI). Larger and more cells (n 100) would give access to a wider linear range for larger surface areasA, beyond the values ACin TableI.

However, the estimated values ofA2of the four acoustic fields are in accordance with the conditionAC A2, since

the minimum value of the ratio AC=A2 is about 100 for

Re½~u; Im½~u; Re½s; and Im½s, for the frequency range between 53 Hz and 2095 Hz (Fig.11).

After having estimated the integral rangeA2of each ran-dom scalar field (Re½uy; Im½uy; Re½s, and Im½s) for the 20

images (Fig.11), we can observe its evolution with the fre-quency of the propagating acoustic wave in the Fig.12.

Figures 12and13show to what extent the integral range A2and the relative precision in estimating the four average scalar fields decrease when the frequency increases for RF¼ 42 lm and RF¼ 100 lm. This can be explained by the

relationship which exists between the frequencyf and the thick-ness of the boundary layer dBL (Eq. (20)), with q0 and g,

respectively, the density and the viscosity of the air filling the pores.1,2Moreover, we can observe on Fig.13that the maximal relative precision of the four scalar fields is about 10%, which is small enough to consider ourn¼ 20 simulations as represen-tative for estimating the average harmonic acoustic fields.

2. RVE of the acoustic fields

The representative volume elements ARVE of the four

acoustic fields can be estimated from the Eq. (25), which depends on the corresponding integral ranges A2 (Fig. 12). The evolution of, the precision of estimation of the average acoustic fields is represented in Fig.14for different represen-tative volume elements ARVE at different scales and

frequencies.

In unit cells composed of small and medium fibres (RF¼ 42 lm; 100 lm), we can notice that the values of ARVE

decrease at fixed precision when the frequency increases (Fig. 14). Therefore, the characteristic sizes of the acoustic

FIG. 11. Estimation of the integral rangeA2from linear regressions made on

VARðhZi_{A}Þ

VARðZÞ for different frequencies. The variable Z is replaced by Re½uy; Im½uy; Re½s, and Im½s. For both uycomponents, the linear

regres-sions are made for the 5 sub-scalesAC;A4C; AC

9; AC

16; and AC

25. For both s compo-nents, the linear regressions are made only for the 3 first sub-scales. RF¼ 42 lm. Logarithmic scales.

fields in unit cells are smaller at high frequencies for RF¼ 42 lm and RF¼ 100 lm, which is consistent with the

decrease of the thickness of the boundary layer at high fre-quencies (Eq. (20)), giving fields with a lower correlation length.

However, the representative volume elements ARVE of

the fields obtained from cells with large fibres (RF¼ 300 lm)

do not seem to evolve with the same monotonic trend as for smaller fibres.

D. Representative volume element of the acoustic absorption

1. Relative precision in the estimation of the acoustic absorption

In order to estimate the relative precision of estima-tion of the acoustic absorpestima-tion with the Eq. (24), the

integral range A2 cannot be estimated, since there is no point varianceVARðZÞ for aðxÞ. However, we can estimate the product VARðZÞ A2 with a linear regression of

VARðhZi_{A}Þ as a function of 1=A (Eq.(23)). Thus, using this
linear regression and the Eq.(24), we obtained the precision
of the acoustic absorption as a function of the total surface
areaA0¼ n ACof our 20 simulations.

The frequential evolution of is represented in Fig.15. We can observe that all the values of are globally smaller than 5% and smaller than the precision of estimation of the average acoustic fields (Fig. 13) for RF¼ 42 lm and

RF¼ 100 lm. Moreover, the values of decrease when both

the thickness d of the material and the frequency increase, for small and medium fibres (RF ¼ 42 lm and 100 lm).

FIG. 12. Evolution of the integral rangeA2withf between 53 Hz and 4032 Hz

forRe½uy; Im½uy; Re½s, and Im½s, at different scales (RF¼ 42 lm; 100 lm; and 300 lm).

FIG. 13. Evolution of the relative precision of estimation with f between 53 Hz and 4032 Hz forhRe½uyi; hIm½uyi; hRe½si; and hIm½si, at different scales (RF¼ 42 lm; 100 lm; and 300 lm). The relative precision was obtained withn¼ 20 independent simulations with a surface area equal to AC(TableI).

For large fibres (RF¼ 300 lm) the fluctuations and the

95% confidence interval previously observed in Fig. 7 are direct consequences of the high values of for the acoustic absorption. This results show that the sizeACof the 20 simu-lations (Table I) is probably not large enough to properly quantify the fluctuation of the acoustic absorption of large

fibres, even if the average value of aðxÞ of the 20 realiza-tions is not very different from the absorption obtained on a deterministic fibre network (orange plots in Fig.7).

2. RVE of the acoustic absorption

Finally, the last step of our work consists in estimating the representative volume element for the acoustic absorp-tion. In Fig.16, we can observe the evolution of the relative precision of estimation of the average value EfaðxÞg with the size A of one simulation of random fibrous media. As a consequence of the results obtained for the acoustic fields (Fig.14), the relative error monotonically decreases (giving a better precision) when the frequency increases for small

FIG. 14. Evolution of the relative precision of estimation ofhRe½uyi; hIm½uyi; hRe½si; and hIm½si over the surface area A of one random realiza-tion (n¼ 1) for RF¼ 42 lm. The minimum surface area A on the Ox axis is equal toACin TableI. Interval between two colored dashed vertical lines:

2 ½1% 5%. Logarithmic scales.

FIG. 15. Evolution of the relative precision with f between 53 Hz and 4032 Hz for the absorption coefficient aðxÞ, at different scales (RF¼ 42 lm; 100 lm; and 300 lm) and for different thicknesses (d¼ 2 cm; 4 cm; and 10 cm). The relative precision was obtained withn¼ 20 independent simula-tions with a surface area equal toAC(TableI).

and medium fibres (RF ¼ 42 lm, 100 lm), for the three

con-sidered thicknesses (d¼ 2 cm; 4 cm; and 10 cm). This is a direct effect of the frequential evolution of the thickness dBL

of the boundary layer (Eq.(20)). This trend is not observable for large fibres (RF¼ 300 lm).

Let us focus on the precision of estimation ofEfaðxÞg over a single simulation composed of small and medium fibres (RF ¼ 42 lm; 100 lm) with a surface area equal to AC (TableI). Even if the maximal value of is equal to 20% at low frequencies (f ¼ 53 Hz), the values of the precision are close to 10% for frequencies higher than 400 Hz (Fig. 16). Therefore, we observe that one unit cell with a surface area equal toACis representative enough to estimate the average absorption coefficient with a precision of 10%, over the fre-quency range between 53 Hz and 2095 Hz. This gives the size of the domain to be used in the random network, to esti-mate the effective acoustic properties with a given precision.

V. CONCLUSIONS

Estimating the acoustic behaviour of random media is a challenging problem, which was recently developed by nu-merical techniques on images of the microstructure. In this

paper is considered the effect of the size of fibres and of their random distribution in space on the acoustic behaviour.

Following a method efficiently applied in the domains of elastostatics and of thermostatics,4,13,17,19,43we extended the statistical determination of the RVE to the harmonic case, in the framework of thermoacoustics. As a result, we are able to estimate the relative precision of estimation of the acoustic properties of porous media, predicted from numeri-cal simulations of the complex harmonic velocity and tem-perature fields in a random medium submitted to an acoustic wave propagation. This precision depends on the scale of calculations, and on the local fluctuations of the fields that can be estimated by numerical techniques. In the present case, thermal properties fluctuate more and develop longer correlation lengths than velocity fields. The thermal proper-ties are therefore the limiting factor to define a representative volume element. The effect of the frequency is to decrease the size of the RVE, as a result of the thinning of the bound-ary layer giving more localized fields.

The method illustrated here on a random fibrous me-dium can be used on more general 3D images or simulations, like foams or granular media, provided the corresponding fields are obtained by numerical calculation.

FIG. 16. Evolution of the relative precision of estimation of the average acoustic absorption EfaðxÞg over the surface area A of one random realization (n¼ 1) at different scales (RF¼ 42 lm; 100 lm; and 300 lm), for thicknesses d equal to 2 cm, 4 cm; and 10 cm, and for f between 53 Hz and 2095 Hz. The minimum surface areaA on the Ox axis is equal to ACin TableI. Interval between two colored dashed vertical lines:2 ½1% 5%. Logarithmic scales.

ACKNOWLEDGMENTS

This work was made as a part of the Silent Wall project (Ref.: ANR-06-MAPR-00-18). We gratefully acknowledge the Agence Nationale de la Recherche (ANR) for its financial support. Moreover, we are grateful to Bernard Castagne`de, Claude Depollier and Olivier Dazel (LAUM, Laboratoire d’Acoustique de l’Universite du Maine, Le Mans, France) for bringing their expert’s point of view in acoustics all along this project.

1

J. F. Allard, Propagation of Sound in Porous Media. Modelling Sound Absorbing Materials (Chapman & Hall, London, 1993).

2_{J. F. Allard, B. Castagne`de, M. Henry, and W. Lauriks, “Evaluation of }

tor-tuosity in acoustic porous materials saturated by air,”Rev. Sci. Instrum.

65, 754–755 (1994).

3

J. F. Allard and Y. Champoux, “New empirical equations for sound propa-gation in rigid frame fibrous materials,” J. Acoust. Soc. Am. 91(6), 3346–3353 (1992).

4

H. Altendorf, “3D Morphological analysis and modeling of random fiber networks,” Ph.D. thesis, Mines ParisTech, 2011.

5_{J. L. Auriault, “Dynamic behaviour of a porous medium saturated by a}

Newtonian fluid,”Int. J. Eng. Sci.18(6), 775–785 (1980).

6

J. L. Auriault, L. Borne, and R. Chambon, “Dynamics of porous saturated media, checking of the generalized law of Darcy,”J. Acoust. Soc. Am.

77(5), 1641–1650 (1985).

7_{J. L. Auriault and E. Sanchez-Palencia, “}_{Etude du comportement }

macro-scopique d’un milieu poreux sature deformable,” J. de Mecanique 16(4), 575–603 (1977).

8_{Y. Champoux and J. F. Allard, “Dynamic tortuosity and bulk modulus in}

air-saturated porous media,”J. Appl. Phys.70(4), 1975–1979 (1991).

9

Y. Champoux and M. R. Stinson, “On acoustical models for sound propa-gation in rigid frame porous materials and the influence of shape factors,”

J. Acoust. Soc. Am.92(2), 1120–1131 (1992).

10_{A. M. Chapman and J. J. L. Higdon, “Oscillatory Stokes flow in periodic}

porous media,”Phys. Fluids A4(10), 2099–2116 (1992).

11

Comsol MultiphysicsTM3.5a,Comsol MultiphysicsTM3.5a-Documentation,

http://www.comsol.com/, 2009.

12_{M. E. Delany and E. N. Bazley, “Acoustical properties of fibrous }

absorb-ent materials,”Appl. Acoust.3, 105–116 (1970).

13

J. Escoda, F. Willot, D. Jeulin, J. Sanahuja, and C. Toulemonde, “Estimation of local stresses and elastic properties of a mortar sample by FFT computation of fields on a 3D image,”Cem. Concr. Res.41, 542–556 (2011).

14

S. Gasser, “Etude des proprietes acoustiques et mecaniques d’un materiau metallique poreux mode`le base de sphe`res creuses de nickel,” Ph.D. thesis, INPG Grenoble, 2003.

15

S. Gasser, F. Paun, and Y. Brechet, “Absorptive properties of rigid porous media: Application to face centered cubic sphere packing,”J. Acoust. Soc. Am.117, 2090–2099 (2005).

16_{D. Jeulin, “Random texture models for materials structures,”} _{Stat.}
Comput.10, 121–131 (2000).

17

D. Jeulin, “Variance scaling of boolean random varieties,” Technical report, Mines ParisTech Publications-HAL-00618967, 2011.

18_{D. L. Johnson, J. Koplik, and R. Dashen, “Theory of dynamic permeability}

and tortuosity in fluid-saturated porous media,” J. Fluid Mech. 176, 379–402 (1987).

19_{T. Kanit, S. Forest, I. Galliet, V. Mounoury, and D. Jeulin, “Determination}

of the size of the representative volume element for random composites: Statistical and numerical approach,”Int. J. Solids Struct.40, 3647–3679 (2003).

20_{D. Lafarge, “Propagation du son dans les mat}

eriaux poreux structure rigide satures par un fluide viscothermique,” Ph.D. thesis, University of the Maine, 1993.

21_{C. Y. Lee, M. J. Leamy, and J. H. Nadler, “Numerical calculation of }

effec-tive density and compressibility tensors in periodic porous media: A multi-scale asymptotic method,” in Proceedings of the COMSOL Conference, Boston, USA, 9–11 October 2008.

22_{C. Y. Lee, M. J. Leamy, and J. H. Nadler, “Acoustic absorption calculation}

in irreducible porous media: A unified computational approach,”

J. Acoust. Soc. Am.126(4), 1862–1870 (2009).

23

G. Matheron, Elements pour une Theorie des Milieux Poreux (Masson, Paris, 1967).

24_{G. Matheron, “The theory of regionalized variables and its applications,”}

Technical report, Mines ParisTech Publications, 1971.

25

F. P. Mechel, “Ausweitung der absorberformel von delany and bazley zu tiefen frequenzen,” Acustica 35, 210–213 (1976).

26_{Y. Miki, “Acoustical properties of porous materials-generalizations of }

em-pirical models,”J. Acoust. Soc. Jpn. (E)11(1), 25–28 (1990).

27

Y. Miki, “Acoustical properties of porous materials-modifications of Delany-Bazley models,” J. Acoust. Soc. Jpn. (E) 11(1), 19–24 (1990).

28

C. Perrot, “Microstructure et macro-comportement acoustique: approche par reconstruction d’une celluleelementaire representative,” Ph.D. thesis, University of Sherbrooke; ENTPE Lyon, 2006.

29_{C. Perrot, F. Chevillotte, M. T. Hoang, G. Bonnet, F. X. B}

ecot, L. Gautron, and A. Duval, “Microstructure, transport, and acoustic properties of open-cell foam samples: Experiments and three-dimensional numerical simulations,”J. Appl. Phys.111, 014911 (2012).

30_{C. Perrot, F. Chevillotte, and R. Panneton, “Bottom-up approach for}

microstructure optimization of sound absorbing materials,”J. Acoust. Soc. Am.124, 940–948 (2008).

31_{C. Perrot, F. Chevillotte, and R. Panneton, “Dynamic viscous permeability}

of an open-cell aluminium foam: Computation versus experiments,”

J. Appl. Phys.103, 024909 (2008).

32

C. Peyrega, “Prediction of the acoustic properties of heterogeneous fibrous materials from their 3D microstructures,” Ph.D. thesis, Mines ParisTech, 2010.

33

C. Peyrega and D. Jeulin, “Effects of the microstructure of fibrous media on their acoustic properties,” in Proceedings of the COMSOL Conference, Versailles, France, 17th–19th November 2010.

34_{C. Peyrega and D. Jeulin, “Simulation of the acoustic behaviour of random}

fibrous materials,” in Proceedings of the Internoise Conference, Osaka, Japan, 4th–7th September 2011.

35_{C. Peyrega, D. Jeulin, C. Delis}

ee, and J. Malvestio, “3D morphological modelling of a random fibrous network,” Image Anal. Stereol. 28, 129–141 (2009).

36

C. Peyrega, D. Jeulin, C. Delisee, and J. Malvestio, “3D morphological characterization of phonic insulation fibrous media,” Adv. Eng. Mater.

13(3), 156–164 (2010).

37

J. Pfretzschner and R. M. Rodrıguez, “Acoustical absorption and critical thickness,” in Proceedings of the 17th International Congress of Acoustics (ICA) 2001, Rome, Italie, 2–7 September 2001.

38_{S. R. Pride, F. D. Morgan, and A. F. Gangi, “Drag forces of porous media}

acoustics,”Phys. Rev. B47(9), 4964–4975 (1993).

39

E. Sanchez-Palencia, “Comportements local et macroscopique d’un type de milieux physiques heteroge`nes,” Int. J. Eng. Sci. 12(4), 331–351 (1974).

40

E. Sanchez-Palencia, Non-Homogeneous Media and Vibration Theory (Springer-Verlag, Heidelberg, 1980).

41_{R. Venegas and O. Umnova, “On the influence of the micro-geometry on}

sound propagation through periodic array of cylinders,” in Proceedings of Acoustics 08, Paris, France, 29th June–4th July 2008, pp. 807–812.

42

R. Venegas and O. Umnova, “Effective acoustical properties of random microfibrous materials,” in Proceedings of Euronoise 2009, Edinburgh, Scotland, 26th–28th October 2009.

43

F. Willot and D. Jeulin, “Elastic behavior of composites containing bool-ean random sets of inhomogeneities,” Int. J. Eng. Sci. 47, 313–324 (2009).

44_{C. Zwikker and C. W. Kosten,} _{Sound Absorbing Materials (Elsevier}

applied sciences, New-York, 1949).